This preview shows page 1. Sign up to view the full content.
Unformatted text preview: SPECIFICATION FOR WELDED UNS N08020, UNS N08024, AND UNS N08026 ALLOY PIPE
(Identical with ASTM Speciﬁcation B 464-99 except that certiﬁcation has been made mandatory.)
01 1. Scope 3. General Requirement 1.1 This speciﬁcation covers welded UNS N08020, N08024, and N08026 alloy pipe for general corrosionresisting and low- or high-temperature service. 1.2 The pipe covered is nominal pipe sizes up to and including NPS 6, with the nominal wall thicknesses given as Schedules 5S, 10S, and 40S and nominal pipe sizes up to and including NPS 2, also including Schedule 80S. Table 2 of Speciﬁcation B 775 is based on Table A1 of ANSI B36.19 and gives the nominal dimensions of these sizes. Table 3 of Speciﬁcation B 775 lists the dimensional requirements of these sizes. Pipe having other dimensions may be furnished provided such pipe complies with all other requirements of this speciﬁcation. 1.3 The values stated in inch-pound units are to be regarded as the standard. The values given in parentheses are for information only. 3.1 Material furnished in accordance with this speciﬁcation shall conform to the applicable requirements of the current edition of Speciﬁcation B 775 unless otherwise provided herein. 4. Ordering Information 4.1 It is the responsibility of the purchaser to specify all requirements that are necessary for the safe and satisfactory performance of material ordered under this speciﬁcation. Examples of such requirements include, but are not limited to, the following: 4.1.1 Quantity (feet or number of lengths), 4.1.2 UNS number, 4.1.3 Size (nominal pipe size and schedule), 4.1.4 Length (random or speciﬁc), 4.1.5 ASTM designation, 4.1.6 Product Analysis — State if required, 4.1.7 Certiﬁcation — Certiﬁcation and a report of test results are required, 4.1.8 Purchaser Inspection — State which tests or inspections are to be witnessed, if any, and 4.1.9 Supplementary requirements, if any. 2. Referenced Documents 2.1 ASTM Standards: A 262 Practices for Detecting Susceptibility to Intergranular Attack in Austenitic Stainless Steels B 775 Speciﬁcation for General Requirements for Nickel and Nickel-Alloy Seamless and Welded Pipe E 8 Test Methods for Tension Testing of Metallic Materials 2.2 ANSI Standard: B36.19 Stainless Steel Pipe
593 5. Materials and Manufacture 5.1 The pipe shall be made from ﬂat-rolled stock by an automatic welding process with no addition of ﬁller metal. COPYRIGHT American Society of Mechanical Engineers Licensed by Information Handling Services SB-464 TABLE 1 CHEMICAL REQUIREMENTS
Composition, % UNS N08020 0.07 2.00 0.045 0.035 1.00 32.00–38.00 19.00–21.00 2.00–3.00 3.00–4.00 8× carbon–1.00 ... Remainder UNS N08024 0.03 1.00 0.035 0.035 0.50 35.00–40.00 22.50–25.00 3.50–5.00 0.50–1.50 0.15–0.35 ... Remainder 2001 SECTION II TABLE 2 MECHANICAL PROPERTY REQUIREMENTS
Tensile Strength, min, ksi (MPa) 80 (551) Yield Strength,A min, ksi (MPa) 35 (241) Elongation in 2 in. (50.8 mm), min, % 30.0 Element Carbon, max Manganese, max Phosphorus, max Sulfur, max Silicon, max Nickel Chromium Molybdenum Copper Columbium (Nb) + tantalum Nitrogen IronA
A UNS N08026 0.03 1.00 0.03 0.03 0.50 33.00–37.20 22.00–26.00 5.00–6.70 2.00–4.00
A Yield strength shall be determined by the offset method at 0.2% limiting permanent set in accordance with Test Methods E 8. An alternative method of determining yield strength may be based on total extension under load of 0.5%. 0.10–0.16 Remainder 6.2 If a product analysis is performed, it shall meet the chemistry limits prescribed in Table 1, subject to the analysis tolerances speciﬁed in Table 1 of Speciﬁcation B 775. 7. Mechanical Properties and Other Requirements By difference. 5.2 Heat Treatment — Pipe of UNS N08020 alloy shall be furnished in the stabilized-annealed condition. Pipe of UNS N08024 alloy shall be furnished in the annealed condition. Pipe of UNS N08026 alloy shall be furnished in the solution-annealed condition.
NOTE 1 — The recommended annealing temperatures are 1800 to 1850°F (982 to 1010°C) for UNS N08020, 1925 to 1975°F (1052 to 1079°C) for UNS N08024, and 2050 to 2200°F (1121 to 1204°C) for UNS N08026. 7.1 Mechanical Properties — The material shall conform to the mechanical property requirements speciﬁed in Table 2. One test is required for each lot as deﬁned in Speciﬁcation B 775. 7.2 Flattening Test — A ﬂattening test shall be made on each end of one pipe per lot. Superﬁcial ruptures resulting from surface imperfections shall not be cause for rejection. 7.3 Nondestructive Test Requirements — Each pipe shall be subjected to either a pressure test or a nondestructive electric test at the manufacturer’s option. The purchaser may specify which test is to be used. 8. Lengths 6. Chemical Composition 6.1 The material shall conform to the composition limits speciﬁed in Table 1. One test is required for each lot as deﬁned in Speciﬁcation B 775. 8.1 Lengths may be ordered as either random lengths (normally 15 to 24 ft (4.6 to 7.3 m) with some agreed upon allowance for shorts) or speciﬁc cut lengths. 594 COPYRIGHT American Society of Mechanical Engineers Licensed by Information Handling Services PART B — NONFERROUS MATERIAL SPECIFICATIONS SB-464 SUPPLEMENTARY REQUIREMENTS
The following supplementary requirements shall be applied only when speciﬁed by the purchaser in the inquiry, contract, or order: S1. Corrosion Tests S1.1 One intergranular corrosion test per lot shall be performed by the manufacturer on a sensitized specimen and tested in accordance with Practices A 262. When this supplementary requirement is speciﬁed, the speciﬁc practice (Practice B or Practice E) shall also be speciﬁed. If Practice B is speciﬁed, the specimen must pass with a rate of less than 0.002 in. (0.05 mm) per month. A lot for intergranular corrosion testing shall be the same as for mechanical testing. S1.1.1 In addition to the anneal recommended in Note 1, the specimen shall be sensitized for 1 h at 1250°F (677°C) before being subjected to corrosion testing. S1.1.2 If any corrosion test specimen fails the test, the material represented by such specimens may be reheat-treated and resubmitted for test. 595 COPYRIGHT American Society of Mechanical Engineers Licensed by Information Handling Services ...
View Full Document
This note was uploaded on 10/04/2010 for the course ENGINEERS 22453175 taught by Professor Heydari during the Spring '08 term at Miami University.
- Spring '08